# Magnetization Reversal in Concave Iron Nano-Superellipses

^{*}

## Abstract

**:**

## 1. Introduction

## 2. Materials and Methods

_{S,Fe}= 1700·10

^{3}A/m as magnetization at saturation, A

_{Fe}= 21·10

^{−12}J/m as exchange constant, and K

_{1,Fe}= 48·10

^{3}J/m

^{3}as cubic magnetocrystalline anisotropy constant [37]. The Gilbert damping constant was 0.5 (quasistatic case), the crystalline orientation was set to constant, with the easy cubic anisotropy axes along 0° and 90° corresponding to epitaxially grown nanostructures. This is in contrast to a previous investigation of square iron nanodots with arbitrary anisotropy orientation per cell [11], to enable investigating the effect of an epitaxial growth in addition to the modification of the sample shape, and thus the shape anisotropy.

_{L}) and transversal magnetization components (M

_{T}) were calculated, and screenshots were taken during the magnetization-reversal processes. The hysteresis loops and six snapshots of the magnetization-reversal process per simulation are depicted in Supplementary Information.

## 3. Results and Discussion

_{C}and reversibility fields H

_{rev}in the angular range of 0°−90°. Values in Figure 6a,c and Figure 6b,d were equal, depicted against the angles of the external magnetic field or the sample number. In most cases, 45° showed the highest coercive field, indicating that this orientation corresponds to an easy axis [41,42,43]. Deviations from this behaviour, as shown in Figure 6c by comparing 0° and 45° for Samples SE10 and SE20, can be attributed to the previously discussed high symmetry of the 0° orientation, which may suppress magnetization reversal, since no rotational direction is favoured by geometry or external magnetic field.

## 4. Conclusions

## Supplementary Materials

## Author Contributions

## Funding

## Institutional Review Board Statement

## Informed Consent Statement

## Data Availability Statement

## Conflicts of Interest

## References

- Reiss, G.; Hütten, A. Applications beyond data storage. Nat. Mater.
**2005**, 4, 725–726. [Google Scholar] [CrossRef] [PubMed] - Harada, M.; Kuwa, M.; Sato, R.; Teranishi, T.; Takahashi, M.; Maenosono, S. Cation Distribution in Monodispersed MFe
_{2}O_{4}(M = Mn, Fe, Co, Ni, and Zn) Nanoparticles Investigated by X-ray Absorption Fine Structure Spectroscopy: Implications for Magnetic Data Storage, Catalysts, Sensors, and Ferrofluids. ACS Appl. Nano Mater.**2020**, 3, 8389–8402. [Google Scholar] [CrossRef] - Poornaprakash, B.; Ramu, S.; Subramanyam, K.; Kim, Y.; Kumar, M.; Reddy, M.S.P. Robust ferromagnetism of ZnO:(Ni + Er) diluted magnetic semiconductor nanoparticles for spintronic applications. Ceram. Int.
**2021**. [Google Scholar] [CrossRef] - Almessiere, M.; Slimani, Y.; Guner, S.; Sertkol, M.; Korkmaz, A.D.; Shirsath, S.E.; Baykal, A. Sonochemical synthesis and physical properties of Co
_{0.3}Ni_{0.5}Mn_{0.2}Eu_{x}Fe_{2−x}O_{4}nano-spinel ferrites. Ultrason. Sonochem.**2019**, 58, 104654. [Google Scholar] [CrossRef] [PubMed] - Esfe, M.H.; Saedodin, S.; Mahian, O.; Wongwises, S. Efficiency of ferromagnetic nanoparticles suspended in ethylene glycol for applications in energy devices: Effects of particle size, temperature, and concentration. Int. Commun. Heat Mass Transf.
**2014**, 58, 138–146. [Google Scholar] [CrossRef] - Barbucci, R.; Pasqui, D.; Giani, G.; De Cagna, M.; Fini, M.; Giardino, R.; Atrei, A. A novel strategy for engineering hydrogels with ferromagnetic nanoparticles as crosslinkers of the polymer chains. Potential applications as a targeted drug delivery system. Soft Matter
**2011**, 7, 5558–5565. [Google Scholar] [CrossRef] - Abu-Bakr, A.F.; Zubarev, A.Y. Effect of ferromagnetic nanoparticles aggregation on magnetic hyperthermia. Eur. Phys. J. Spec. Top.
**2020**, 229, 323–329. [Google Scholar] [CrossRef] - Slimani, Y.; Unal, B.; Hannachi, E.; Selmi, A.; Almessiere, M.A.; Nawaz, M.; Baykal, A.; Ercan, I.; Yildiz, M. Frequency and dc bias voltage dependent dielectric properties and electrical conductivity of BaTiO
_{3}-SrTiO_{3}/(SiO_{2})_{x}nanocomposites. Ceram. Int.**2019**, 45, 11989–12000. [Google Scholar] [CrossRef] - Mejía-López, J.; Altbir, D.; Romero, A.H.; Batlle, X.; Roshchin, I.V.; Li, C.-P.; Schuller, I.K. Vortex state and effect of anisotropy in sub-100-nm magnetic nanodots. J. Appl. Phys.
**2006**, 100, 104319. [Google Scholar] [CrossRef] [Green Version] - Noske, M.; Stoll, H.; Fähnle, M.; Gangwar, A.; Woltersdorf, G.; Slavin, A.; Weigand, M.; Dieterle, G.; Förster, J.; Back, C.H.; et al. Three-dimensional character of the magnetization dynamics in magnetic vortex structures: Hybridization of flexure gyromodes with spin waves. Phys. Rev. Lett.
**2016**, 117, 037208. [Google Scholar] [CrossRef] [PubMed] [Green Version] - Ehrmann, A.; Blachowicz, T. Systematic study of magnetization reversal in square Fe nanodots of varying dimensions in different orientations. Hyperfine Interact.
**2018**, 239, 48. [Google Scholar] [CrossRef] - Ehrmann, A.; Blachowizc, T. Vortex and double-vortex nucleation during magnetization reversal in Fe nanodots of different dimensions. J. Magn. Magn. Mater.
**2019**, 475, 727–733. [Google Scholar] [CrossRef] - Döpke, C.; Grothe, T.; Steblinski, P.; Klöcker, M.; Sabantina, L.; Kosmalska, D.; Blachowicz, T.; Ehrmann, A. Magnetic Nanofiber Mats for Data Storage and Transfer. Nanomaterials
**2019**, 9, 92. [Google Scholar] [CrossRef] [PubMed] [Green Version] - Almessiere, M.; Slimani, Y.; Güner, S.; Nawaz, M.; Baykal, A.; Aldakheel, F.; Akhtar, S.; Ercan, I.; Belenli, I.; Ozçelik, B. Magnetic and structural characterization of Nb
^{3+}-substituted CoFe_{2}O_{4}nanoparticles. Ceram. Int.**2019**, 45, 8222–8232. [Google Scholar] [CrossRef] - Almessiere, M.; Slimani, Y.; Korkmaz, A.; Taskhandi, N.; Sertkol, M.; Baykal, A.; Shirsath, S.E.; Ercan, I.; Ozçelik, B. Sonochemical synthesis of Eu3+ substituted CoFe
_{2}O_{4}nanoparticles and their structural, optical and magnetic properties. Ultrason. Sonochem.**2019**, 58, 104621. [Google Scholar] [CrossRef] [PubMed] - Sathisha, I.C.; Manjunatha, K.; Angadi, V.J.; Reddy, R.K. Structural, Microstructural, Electrical, and Magnetic Properties of CuFe
_{2-(x + y)}EuxSc_{y}O_{4}(where x and y vary from 0 to 0.03) Nanoparticles. J. Supercond. Novel Magn.**2020**, 33, 3963–3973. [Google Scholar] [CrossRef] - Kasperski, M.; Puszkarski, H.; Hoang, D.-T.; Diep, H.T. Magnetic properties of two-dimensional nanodots: Ground state and phase transition. AIP Adv.
**2013**, 3, 122121. [Google Scholar] [CrossRef] [Green Version] - Vavassori, P.; Zaluzec, N.; Metlushko, V.; Novosad, V.; Ilic, B.; Grimsditch, M. Magnetization reversal via single and bouble vortex states in submicron Permalloy ellipses. Phys. Rev. B
**2004**, 69, 214404. [Google Scholar] [CrossRef] [Green Version] - Guslienko, K.Y.; Buchanan, K.S.; Bader, S.D.; Novosad, V. Dynamics of coupled vortices in layered magnetic nanodots. Appl. Phys. Lett.
**2005**, 86, 223112. [Google Scholar] [CrossRef] [Green Version] - Prosandeev, S.; Bellaiche, L. Controlling Double Vortex States in Low-Dimensional Dipolar Systems. Phys. Rev. Lett.
**2008**, 101, 097203. [Google Scholar] [CrossRef] [PubMed] [Green Version] - Vavassori, P.; Grimsditch, M.; Novosad, V.; Metlushko, V.; Ilic, B. Metastable states during magnetization reversal in square permalloy rings. Phys. Rev. B
**2003**, 67, 134429. [Google Scholar] [CrossRef] - Remhof, A.; Schumann, A.; Westphalen, A.; Last, T.; Kunze, U.; Zabel, H. Dipolar interactions in periodic arrays of rectangular ferromagnetic islands. J. Magn. Magn. Mater.
**2007**, 310, e794–e796. [Google Scholar] [CrossRef] - Zabel, H.; Schumann, A.; Westphalen, A.; Remhof, A. Order and Frustration in Artificial Magnetic Patterns. Acta Phys. Pol. A
**2009**, 115, 59–63. [Google Scholar] [CrossRef] - Gao, X.; Liu, L.; Birajdar, B.; Ziese, M.; Lee, W.; Alexe, M.; Hesse, D. High-Density Periodically Ordered Magnetic Cobalt Ferrite Nanodot Arrays by Template-Assisted Pulsed Laser Deposition. Adv. Funct. Mater.
**2009**, 19, 3450–3455. [Google Scholar] [CrossRef] - Li, Z.; Gao, S.; Brand, U.; Hiller, K.; Hahn, S.; Hamdana, G.; Peiner, E.; Wolff, H.; Bergmann, D. Nanomechanical character-ization of vertical nanopillars using an MEMS-SPM nano-bending testing platform. Sensors
**2019**, 19, 4529. [Google Scholar] [CrossRef] [PubMed] [Green Version] - Ehrmann, A.; Blachowicz, T.; Komraus, S.; Nees, M.-K.; Jakobs, P.-J.; Leiste, H.; Mathes, M.; Schaarschmidt, M. Magnetic properties of square Py nanowires: Irradiation dose and geometry dependence. J. Appl. Phys.
**2015**, 117, 173903. [Google Scholar] [CrossRef] - Blachowicz, T.; Ehrmann, A.; Steblinski, P.; Palka, J. Directional-dependent coercivities and magnetization reversal mechanisms in fourfold ferromagnetic systems of varying sizes. J. Appl. Phys.
**2013**, 113, 013901. [Google Scholar] [CrossRef] [Green Version] - Huang, W.W.; Li, Y.Y.; Niklas, K.J.; Gielis, J.; Ding, Y.Y.; Cao, L.; Shi, P.J. A superellipse with deformation and its application in describing the cross-sectional shapes of a square bamboo. Symmetry
**2020**, 12, 2073. [Google Scholar] [CrossRef] - Castán-Guerrero, C.; Herrero-Albillos, J.; Bartolomé, J.; Rodríguez, L.A.; Magén, C.; Kronast, F.; Gawronski, P.; Chubykalo-Fesenko, O.; Merazzo, K.J.; Vavassori, P.; et al. Magnetic antidot to dot crossover in Co and Py nanopatterned thin films. Phys. Rev. B
**2014**, 89, 144405. [Google Scholar] [CrossRef] [Green Version] - Sudsom, D.; Ehrmann, A. Micromagnetic Simulations of Fe and Ni Nanodot Arrays Surrounded by Magnetic or Non-Magnetic Matrices. Nanomaterials
**2021**, 11, 349. [Google Scholar] [CrossRef] - Janutka, A.; Gawronski, P. Spin-Transfer Driven Dynamics of Magnetic Vortices and Antivortices in Dots with Crystalline Cubic Anisotropy. IEEE Trans. Magn.
**2017**, 53, 1. [Google Scholar] [CrossRef] - Wang, H.; Campbell, C.E. Spin dynamics of a magnetic antivortex: Micromagnetic simulations. Phys. Rev. B
**2007**, 76, 220407. [Google Scholar] [CrossRef] [Green Version] - Xing, X.J.; Yu, Y.P.; Wu, S.X.; Xu, L.M.; Li, S.W. Bloch-point-mediated magnetic antivortex core reversal triggered by sudden excitation of a suprathreshold spin-polarized current. Appl. Phys. Lett.
**2008**, 93, 202507. [Google Scholar] [CrossRef] - Gliga, S.; Hertel, R.; Schneider, C.M. Switching a magnetic antivortex core with ultrashort field pulses. J. Appl. Phys.
**2008**, 103, 7. [Google Scholar] [CrossRef] - Gliga, S.; Yan, M.; Hertel, R.; Schneider, C.M. Ultrafast dynamics of a magnetic antivortex: Micromagnetic simulations. Phys. Rev. B
**2008**, 77, 060404. [Google Scholar] [CrossRef] [Green Version] - Donahue, M.J.; Porter, D.G. OOMMF User’s Guide, Version 1.0; National Institute of Standards and Technology (NIST): Gaithersburg, MD, USA, 1999. [Google Scholar]
- Kneller, E.F.; Hawig, R. The exchange-spring magnet: A new material principle for permanent magnets. IEEE Trans. Magn.
**1991**, 27, 3588–3560. [Google Scholar] [CrossRef] - Tillmanns, A.; Blachowicz, T.; Fraune, M.; Güntherodt, G.; Schuller, I.K. Anomalous magnetization reversal mechanism in unbiased Fe/FeF2 investigated by means of the magneto-optic Kerr effect. J. Magn. Magn. Mater.
**2009**, 321, 2932–2935. [Google Scholar] [CrossRef] - Blachowicz, T.; Ehrmann, A. Exchange Bias in Thin Films—An Update. Coatings
**2021**, 11, 122. [Google Scholar] [CrossRef] - Detzmeier, J.; Königer, K.; Blachowicz, T.; Ehrmann, A. Asymmetric hysteresis loops in structured ferromagnetic nanoparticles with hard/soft areas. Nanomaterials
**2021**, 11, 800. [Google Scholar] [CrossRef] [PubMed] - Grimsditch, M.; Hoffmann, A.; Vavassori, P.; Shi, H.T.; Lederman, D. Exchange-induced anisotropies at ferromagnetic-antiferromagnetic interfaces above and below the Néel temperature. Phys. Rev. Lett.
**2003**, 90, 257201. [Google Scholar] [CrossRef] [PubMed] - Pardavi-Horvath, M.; Ross, C.; McMichael, R. Shape effects in the ferromagnetic resonance of nanosize rectangular permalloy arrays. IEEE Trans. Magn.
**2005**, 41, 3601–3603. [Google Scholar] [CrossRef] - Blachowicz, T.; Tillmanns, A.; Fraune, M.; Ghadimi, R.; Beschoten, B.; Güntherodt, G. Exchange bias in epitaxial CoO/Co bilayers with different crystallographic symmetries. Phys. Rev. B
**2007**, 75, 054425. [Google Scholar] [CrossRef]

**Figure 1.**Sketches of some shapes under examination: (

**a**) SE0; (

**b**) SE20; (

**c**) SE40; (

**d**) SE60; and (

**e**) SE90; (

**f**) definition of angles in this study.

**Figure 2.**(

**a**,

**c**,

**e**) Hysteresis loops and (

**b**,

**d**,

**f**) snapshots of the magnetization reversal from positive to negative saturation and back, simulated for SE0 at angles defined in the graphs.

**Figure 3.**(

**a**,

**c**,

**e**) Hysteresis loops and (

**b**,

**d**,

**f**) snapshots of magnetization reversal from positive to negative saturation and back, simulated for Sample SE20 at angles defined in the graphs.

**Figure 4.**(

**a**,

**c**) Hysteresis loops and (

**b**,

**d**) snapshots of magnetization reversal from positive to negative saturation and back, simulated for SE30 at angles defined in the graphs.

**Figure 5.**(

**a**,

**c**,

**e**) Hysteresis loops and (

**b**,

**d**,

**f**) snapshots of magnetization reversal from positive to negative saturation and back, simulated for SE50 at angles defined in the graphs.

**Figure 6.**(

**a**,

**c**) Coercive fields and (

**b**,

**d**) reversibility fields as function of (

**a**,

**b**) the angle of the external magnetic field or (

**c**,

**d**) the sample number, respectively.

Publisher’s Note: MDPI stays neutral with regard to jurisdictional claims in published maps and institutional affiliations. |

© 2021 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (https://creativecommons.org/licenses/by/4.0/).

## Share and Cite

**MDPI and ACS Style**

Öncü, E.; Ehrmann, A.
Magnetization Reversal in Concave Iron Nano-Superellipses. *Condens. Matter* **2021**, *6*, 17.
https://doi.org/10.3390/condmat6020017

**AMA Style**

Öncü E, Ehrmann A.
Magnetization Reversal in Concave Iron Nano-Superellipses. *Condensed Matter*. 2021; 6(2):17.
https://doi.org/10.3390/condmat6020017

**Chicago/Turabian Style**

Öncü, Emre, and Andrea Ehrmann.
2021. "Magnetization Reversal in Concave Iron Nano-Superellipses" *Condensed Matter* 6, no. 2: 17.
https://doi.org/10.3390/condmat6020017